Download presentation

Presentation is loading. Please wait.

Published byTess Burkley Modified over 3 years ago

1
**Acero 2000 PHYSICAL METALLURGY AND THERMAL PROCESSING OF STEEL**

Ernesto Gutierrez-Miravete Rensselaer at Hartford Monterrey, Mexico, Julio, 2000

2
**Course Outline 1.- Physical Metallurgy of Steel**

2.- Phase Transformations in Steel 3.- Solidification of Steel 4.- Heat Treatment of Steel 5.- Welding and Surface Treatment of Steel 6.- Supplementary Reading

3
**1.- Physical Metallurgy of Steel**

1.1.- Iron 1.2.- Iron-Carbon Alloys 1.3.- Steels

4
1.1.- Iron Thermodynamic Properties Phases Crystal Structures

5
**1.2.- Iron-Carbon Alloys Crystal Structures Phases and Microstructures**

Thermodynamic Properties Phase Diagram

6
**1.3.- Steels Alloying Elements Phase Diagrams Thermodynamic Properties**

Structural Effects Diffusion Real Surfaces

7
**Iron, Iron Alloys and Fe-C system**

Medium of first transition series: Ar3d64s2 Earth Crust contains ~ 4% Fe Tf =1540 C ; Th ~ 750 C Useful Phase Transformations (bcc-fcc) Ferromagnetic below 768 C

8
**Iron, Iron Alloys and Fe-C system (contd)**

Interstitials: H, B, C, N, O Substitutionals: Mostly transition series left, right and below of Fe Fe-C system is the basis of steel metallurgy

9
**Phases and Phase Diagrams**

Equilibrium Phases Ferrite (: T < 906, : 1401 < T <1540 C) Austenite (: 906 C < T < 1401 C) Liquid (l: T > 1540 C) Carbide, Nitride, Oxide Compounds Phase Diagrams Graphic display of stable phases as function of temperature.

10
**Crystalline Structures, Microconstituents and Microstructures**

Equilibrium Crystal Stuctures Ferrite (Body Centered Cubic; BCC) Austenite (Face Centered Cubic; FCC) Carbides, Nitrides, Oxides (Complex)

11
**Crystalline Structures, Microconstituents and Microstructures (contd)**

Equilibrium Microconstituents Ferrite Austenite Pearlite (Ferrite-Carbide Micro-Composite)

12
**Crystalline Structures, Microconstituents and Microstructures (contd)**

Equilibrium Microstructures Ferrite (Grains, Allotriomorphs, Widmanstatten Side-Plates) Austenite (Grains - Twinned) Pearlite (Ferrite-Carbide Colonies)

13
**Crystal Defects Vacancies Dislocations Stacking Faults**

Nv = C exp(- U/kT) Dislocations -Fe (a/2)<111> -Fe (a/2)<110> Stacking Faults -Fe High SFE -Fe Low SFE ( Twinning)

14
**Crystal Defects (contd)**

Grain Boundaries Low Angle High Angle Interstitial and Substitutional Atoms Interphase Interfaces Coherent Semi-coherent Incoherent

15
**Crystal Defects (contd)**

Gibbs-Thompson Equation ln (c(r)/c) = 2 V/r R T Surfaces Crystalline arrangement Surface strain Chemical layering

16
**Multilayer Structure of Real Surfaces**

Steel Decarburized steel Steel-Oxide transition zone Wustite layer Magnetite layer Haematite layer

17
**Effects of Alloying Elements**

Physico-chemical properties Mechanical properties Magnetic properties Corrosion resistant properties

18
**Alloying Elements Expanded -field Contracted -field**

Open (Ni, Co, Mn, Ru, Rh, Os, Ir, Pt) Compunds (C, N, Cu, Zn, Au) Contracted -field Closed (Si, Al, Be, P, Ti, V, Mo, Cr) Compounds (Ta, Nb, Zr)

19
**2.- Phase Transformations in Steel**

2.1.- Temperature-Time Charts 2.2.- Mathematical Modeling of Thermal Processing of Steel 2.3.- Phase Transformations during Cooling 2.4.- Phase Transformations during Heating 2.5.- Research Techniques

20
**2.1.- Temperature-time Charts**

Casting and Cooling of Liquid Steel Heat Treating Thermomechanical Processing

21
**2.2.- Mathematical Modeling of Thermal Processing of Steel**

Diffusion Heat Transfer Fluid and Solid Mechanics Electromagnetism Microstructural Evolution

22
**2.3.- Phase Transformations during Cooling**

Solidification Pearlite Formation Ferrite Formation Cementite Formation Bainite Formation Martensite Formation

23
**2.4.- Phase Transformations during Heating**

Recrystallization Austenitization Tempering Melting

24
**2.5.- Research Techniques Metallography Microscopy Crystallography**

Mechanical Testing Thermometry Mathematical Modeling

25
**Phase Transformations**

Continuum Rate Equations: Convection, Difusion of Mass, Energy and Electromagnetic Fields, Kinetics Phase Transformation Kinetics Additional Microconstituents Isothermal and Continuous Cooling Transformation Diagrams

26
**Continuum Rate Equations**

Conservation of Mass (Eqn. of Continuity) Conservation of Momentum (Eqn. of Motion) Conditions of Compatibility Conservation of Energy (Energy Eqn.)

27
**Continuum Rate Equations (contd)**

Conservation of Species (Diffusion Eqn. and/or Convection/Diffusion Eqn.) Maxwell’s Equations Constitutive Equations Boundary Conditions Arrhenius Rate Equation r = A exp(- E/kT)

28
**Phase Transformation Kinetics**

Diffusive Nucleation-Growth Transformations f = (4/3) Sot I G3 (t - )3 d f = 1 - exp(- a tb) Displacive Transformations (T < Ms) f = max {1 - exp( - K0 [Ms - T])} Diffusive-Displacive Transformations

29
**Phase Transformation Kinetics (contd)**

Grain Growth ( d = grain diameter) d/t = K1 exp(-Q/k T) d (1 - 1/n) Precipitate Growth/Dissolution (diffusion controlled) ( r = precipitate radius) r/t = {2 D V c / r R T}{ 1/rm - 1/r}

30
**Phase Transformation Kinetics (contd)**

Precipitate Growth/Dissolution (interface controlled) r/t = {2 K2 V c/ R T}{ 1/rm - 1/r} Analytical solution (dilute solution) r2 - ro2 = 2 a C D t where C = (ci - ce)/(cp-ce) << 1 and a = 1 + ro/( D t) 1/2

31
**Phase Transformation Kinetics (contd)**

Solute balance at a steady state moving solid-liquid interface - D (c/x) = V (cL* - cS*) = V co (1/k - 1) i.e. c(x) = co + co (1/k - 1) exp[ - V x/D] Solid-liquid interface stability condition G < m Gc = m V (cL* - cS*)/ D

32
**Phase Transformation Kinetics (contd)**

Dendritic growth (primary spacing) 1 = K3 /V1/4 G 1/2 Dendritic growth (secondary spacing) 2 = K4 ts1/3 Eutectic growth (interlamellar spacing) e = K5 V1/2

33
**Non-Equilibrium Microconstituents**

Martensite Body Centered Tetragonal; BCT C-supersaturated Ferrite Laths, Plates, Needles Bainite BCC-BCT Ferrite-Carbide Micro-Composite Laths, Plates

34
**Isothermal Transformation Diagrams**

path 1 path 2 path 3 t

35
**Continuous Cooling Transformation Diagrams**

path 1 path 3 path 2 t

36
**Properties of Individual Microconstituents in Steel**

High-purity Ferrite (single crystal) Theoretical yield shear stress ~ 2000 MPa Actual yield shear stress ~ 10 MPa High-purity Ferrite (polycrystal) Theoretical yield shear stress ~ 6000 MPa Actual yield shear stress ~ MPa Grain size dependence = o +K /d1/2

37
**Properties of Individual Microconstituents in Steel (contd)**

Pearlite Yield strength MPa Tensile strength MPa Bainite Yield strength MPa Tensile strength MPa Martensite Yield strength MPa

38
**Steel as a Composite Material**

Rule of Mixtures = a fa + b fb Empirical relations (low C steel) = 15.4 { (%Mn) + 5.4 (%Si) (%pearlite) + 0.5/d 1/2}

39
**Steel as a Composite Material (contd)**

Empirical relations (eutectoid steel) = /d1/2 where d = interlamellar spacing (mm)

40
**Strengthening Mechanisms in Steel**

Solid Solution Strengthening Dispersion Hardening Dislocation Strengthening Grain Boundary Strenghening

41
**Thermal Processing Techniques and Thermometry**

Heating and Cooling Induction and Resistance Heaters High Energy Density Beams Molds Quenching Baths Thermometry and Dilatometry Temperature Measurement Volume Measurement

42
**Diffractometry/Quantitative Metallography/Image Analysis**

X-Rays Electrons Neutrons Microscopy Optical Electron Field Ion

43
**Diffractometry/ Quantitative Metallography/Image Analysis (contd)**

Image acquisition Digital processing Thresholding operations Mathematical morphology operations Measurements

44
Mechanical Testing Hardness test Tensile test Creep test Fracture test Fatigue test

45
**Mathematical Modeling and Computer Simulation**

Hardware PC Workstations Supercomputers Software Custom -made Research Commercial

46
**Reading Verhoeven et al, JOM, Sept 1998**

Sundman & Agren, MRS Bull, Apr 1999

47
**3.- Thermal Processing of Liquid Steel**

3.1.- Liquid-Solid Transformations 3.2.- Microstructure Formation during Solidification 3.3.- Macrostructure Formation during Solidification 3.4.-Mathematical Modeling of Steel Solidification

48
**3.1.- Liquid-Solid Transformations**

Melting and Solidification of Pure Iron Solidification of Liquid Steel to Primary Delta-Ferrite Solidification of Liquid Steel to Primary Austenite Melting of Alloy Additions in Liquid Steel

49
**3.2.- Microstructure Formation during Solidification**

Nucleation of Crystals Dendritic Growth The Peritectic Transformation during Steel Solidification Microsegregation

50
**3.3.- Macrostructure Formation during Solidification**

Formation and Evolution of the Mushy Zone during Solidification of Steel Solute Transport and Settling/Floating of Crystals in the Melt Macrosegregation Contraction during Solidification Stresses from Solidification

51
**3.4.-Mathematical Modeling of Steel Solidification**

Heat Transfer Solute Transport Microstructural Evolution Stress Generation

52
**Reading Vanaparthy & Srinivasan, Mod. & Sim. in MSE, Vol. 6, 1998**

Schwerdtfeger at al, Met & Matls Trans B, Oct 1998

53
**4.- Heat Treating of Steel**

4.1.- Hardenability 4.2.- Austenitizing 4.3.- Annealing 4.4.- Quenching 4.5.- Tempering 4.6.- Mathematical Modeling

54
**4.1.- Hardenability Concept of Hardenability**

Physical Foundation of Hardenability Measurement of Hardenability Influence of Hardenability on Structure and Properties

55
4.2.- Austenitizing Nucleation and Growth of Austenite during Austenitization Dissolution of Carbides during Austenitization Austenite Grain Growth during Austenitization

56
**4.3.- Annealing Phase Transformations during Isothermal Holding**

Nucleation and Growth of Ferrite Nucleation and Growth of Pearlite Nucleation and Growth of Cementite

57
**4.4.- Quenching Phase Transformations during Continuous Cooling**

Nucleation and Growth of Bainite The Martensitic Transformation Formation of Composite Microstructures containing Multiple Microconstituents Dimensional Changes

58
**4.5.- Tempering Precipitation and Growth of Carbides during Heating**

Transformation of Retained Austenite during Heating Change of Physical Properties during Tempering Dimensional Changes

59
**4.6.- Mathematical Modeling of Heat Treatment of Steel**

Heat Transfer Solute Transport Microstructure Evolution Stress Generation

60
**Reading Homberg, Acta Mater. Vol. 44, 1996**

Inoue & Arimoto, J. Matls Eng. & Perf., Feb 1997 Archambault et al, J. Matls Eng. & Perf., Feb 1997

61
**5.- Welding and Surface Treatment of Steel**

5.1.- Welding of Steel 5.2.- Case Hardening of Steel 5.3.- Surface Hardening by Rapid Heating and Cooling

62
**5.1.- Welding of Steel Welding Process**

Weld Microstructure and Properties Mathematical Modeling

63
**5.2.- Case Hardening of Steel**

Case Hardening Processes Solute Diffusion from the Surface of Steel Decarburization of Steel on Heating Nitriding Mathematical Modeling

64
**5.3.- Surface Hardening by Rapid Heating and Cooling**

Diffusion of Time-Varying Electromagnetic Fields into Steel Surface Heating by Eddy Currents Surface Heating by Focused Beams Phase Transformations during Rapid Surface Heating Mathematical Modeling

65
**Reading Mundra et al, Weld. J. WRS, Apr 1997 Bhadeshia, 1999**

Mittemeijer & Somers, Surf. Eng, Vol. 13, 1997 Fuhrmann & Homberg, 1999

Similar presentations

OK

Fe-Carbon Diagram, TTT Diagram & Heat Treatment Processes

Fe-Carbon Diagram, TTT Diagram & Heat Treatment Processes

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Module architecture view ppt on iphone Ppt online form date Ppt on andhra pradesh Ppt on db2 introduction to economics Ppt on decimals for class 5 Ppt on electronic configuration of elements Ppt on history of prime numbers Ppt on non farming activities Ppt on human resources planning Ppt online viewership